Abstract
Thermal resistance at interfaces and grain boundaries is important in a range of fields from microelectronics to energy materials. Standard models treat interfaces as structureless even though at the nanoscale they are often better described as arrays of linear defects. Here, we examine several characteristics of heat transport that arise when considering such a structure at the interface. When heat carrying phonons scatter off linear defect arrays, diffraction of phonons occurs. Furthermore, a dimensionality crossover is observed in diffusive transport. Phonons transition from seeing a structureless planar defect when their wavelength is longer than the defect spacing, \(\lambda \gtrsim D\), to seeing the interface as a collection of independently scattering linear defects when \(\lambda \lesssim D\). By applying this theory to grain boundary strainfield scattering, we show that this dimensionality crossover can explain the frequency dependence of grain boundary scattering and transmissivity, which results in the T^{2} temperature dependence observed in the lowT thermal conductivity of poly/nanocrystalline materials.
Introduction
Heat conduction across interfaces is an inherently complicated topic of great scientific and technological importance. Advancement in microelectronic technologies (e.g. microprocessors, highpower electronics^{1}) demands ever more efficient removal of the heat generated^{2,3}, making the reduction of phonon scattering at interfaces an important engineering challenge. In the opposite direction, maximizing phonon scattering by interfacial defects is essential for engineering thermal transport in stateoftheart thermal barrier coatings^{4,5}, and thermoelectrics^{6,7}.
The current standard models for describing phononinterface interactions are the acoustic and diffuse mismatch models (AMM and DMM)^{8}, which define the interface as a structureless planar defect where the transmissivity or scattering rate is determined by the bulk properties on either side of the interface. Specifically, within the AMM phonons interact with interfaces through an acoustic analog of the refraction of light, where a change in elastic properties (i.e. acoustic impedance) determines the probability that an incident phonon will reflect or transmit across the interface^{9,10}. In the DMM every phonon scatters randomly or diffusely at the interface and the probability of transmission is determined by the density of phonon states on either side of the boundary^{10}. The commonly used gray model also assumes diffuse scattering and simply limits the phonon mean free path (MFP) to the average grain size of a polycrystal. This is essentially an extension of the Casmir limit which was initially proposed for single crystals where the MFP was limited to the size of the sample^{11}. Each of these models predicts frequency independent scattering of phonons at low temperatures, and thus predicts a T^{3} temperature dependence in the lattice thermal conductivity, κ_{L}, stemming from the temperature dependence of the heat capacity.
In contrast, studies of the lowT κ_{L} of polycrystals provided by Wang et al.^{12}, Watari et al.^{13}, and Berman^{14} show a κ_{L} ∝ T^{2} temperature dependence (Fig. 1) which is characteristic of a grain boundary (GB) scattering rate that is linear in frequency, τ^{−1} ∝ ω. An empirical expression for the spectral transmissivity function of phonons at GBs with the form t(ω) = (1 + αω/ω_{max})^{−1} (where α is a constant on the order of unity, and ω_{max} is the maximum phonon frequency), was presented to account for the observed κ_{L} ∝ T^{2} (τ^{−1} ∝ ω) behavior in polycrystals^{12} and has been used in a number of computational and experimental studies^{15,16,17}. Additionally, Hua et al.^{18} have recently measured the spectral phonon transmissivity of an Al–Si interface and experimentally showed that the interface of dissimilar materials can have a transmissivity function which is ωindependent at the lowest frequencies and decreases above some critical crossover frequency^{18}. Providing mechanistic explanations for these phenomena is a key step in understanding phononinterface interactions at a fundamental level.
The frequency independence of the phonon scattering in the AMM, DMM, and grey models stems (in part) from their definition of the interface as a structureless planar defect. However, real interfaces between similar (GBs) and dissimilar (phase boundaries) materials are not structureless at the nanoscale but are better described as arrays of linear defects of various types (refs.^{19,20,21,22,23,24} and Section 2.3 of ref. ^{25}). In fact, prevailing models of GB defect energies and structure have essentially extended the classic Read–Shockley model^{24}, which defines the GB structure as an array of lattice dislocations, to many GB types (including GBs at high angle) despite the complexity and variety of GB structures^{26,27,28}. Further, interfaces between dissimilar materials are known to accommodate the mismatch in lattice parameter by the formation of arrays of misfit dislocations spaced periodically (e.g. GaAs heterostructures^{29,30}). XRay and electron diffraction peaks arising from the periodic dislocation structures in semicoherent phase boundaries and GBs have been experimentally observed and can be used to study interfacial structure^{31,32}. We note that the wavelength of Xrays and electrons used in these studies are comparable to the wavelengths of heat carrying phonons. The interface between two crystalline materials with structural periodicity will tend to have structural periodicity itself. We propose that the description of phononinterface scattering should be grounded in a definition which contains this structural information.
Phonon diffraction conditions arising from periodically spaced dislocations have been discussed previously by authors, such as Klemens^{33}, Carruthers^{34}, and are formally considered by Omini and Sparavigna^{35}. Previous works, however, have not examined the dimensionality crossover effects that diffraction engenders. We have previously suggested that dislocation strain may dominate phononGB scattering processes^{36}. Here we develop a rigorous theory for this and identify several interesting phenomena that arise from treating the GB dislocation arrays collectively. (This study focuses only on phononinterface interactions, and does not consider electron–phonon interactions which can be important at metal–semiconductor interfaces).
To that end, we first discuss the general effect of defect dimensionality on phonon scattering in order to establish concepts that will be used to interpret the theory that follows. We then derive a general formula to calculate the phonon lifetime due to an array of linear defects, where by analyzing the conservation laws and kinematics of this system, diffraction conditions, and a crossover in defect dimensionality can be observed. Next, this general formula is applied to the specific case of phononGB strain field scattering by defining the linear defects as the strain field from edge dislocations which collectively define a symmetric tilt GB. A simple, semiempirical expression is provided as an excellent approximation of the full analytical theory which embodies the crossover in defect dimensionality observed in this calculation. Finally, this scattering theory is applied to standard phonon transport models, where the phononGB strain field scattering and inherent dimensionality crossover provide a mechanistic explanation for the experimentally observed κ_{L} ∝ T^{2} of polycrystalline and nanocrystalline materials^{12,13,14}. This power law analysis provides evidence that the dominate phononGB scattering mechanism is through GB strain fields. It may also provide an explanation for crossover effects in the frequency dependence of phonon transmissivity at phase boundary interfaces^{18}.
Results
Dimensionality and phonon scattering rate
We start by considering the effect of just the dimensionality of the scattering defect on the ωdependence of the phonon lifetime. We follow the basic precepts of the theory of phonon scattering and its contribution to lattice thermal conductivity as laid out, for example, by Ziman^{37}. By applying these precepts to elastic scattering from a defect with scattering potential V (described in more detail in Supplementary Note 1), the scattering rate or inverse lifetime (Γ(k) = τ(k)^{−1}) of a phonon with wavevector k and frequency ω may be written as a product of three factors,
The three factors n, g, and \(\overline {\left M \right^2}\) are the spatial density of the defect in the crystal, the phonon density of states (pDOS), and a term containing the square of a scattering matrix element \(M = \left\langle {{\mathbf{k}}^\prime \left {{\cal H}^\prime } \right{\mathbf{k}}} \right\rangle = (L_xL_yL_z)^{  1}{\int} {\mathrm {d}}^3{\mathbf{r}}{\kern 1pt} V({\mathbf{r}}){\mathrm {e}}^{i({\mathbf{k}}  {\mathbf{k}}^\prime ) \cdot {\mathbf{r}}}\), where V(r) is the scattering potential and L_{x}L_{y}L_{z} is the volume of the crystal containing the defect. The bar in \(\overline {\left M \right^2}\) indicates that M^{2} has been weighted by the forward scattering parameter and summed over possible final states k′. The essential point, indicated by the subscript ‘\(\bar n\mathrm{d}\)’, is that all three factors depend on \(\bar n\), the codimension of the defect. That is,
with d_{d} being the dimensionality of the defect. Thus, for a onedimensional defect such as a dislocation line, d_{d} = 1 and \(\bar n = 2\), for a point defect d_{d} = 0 and \(\bar n = 3\), and so on.
We can understand Eq. (1) as follows. For example consider a line defect, so \(\bar n = 2\). Suppose the defect is parallel to the zaxis. Then, in addition to the energy, the z component of the phonon wavevector must also be conserved in the scattering event. This results in the phonon scattering onto a circle in k space, and when summing over all possible final state wavevectors the density of accessible phonon states is effectively that of a system with two real spatial dimensions, written as g_{2d}. At the same time, the matrix element of the perturbation reduces to an integral over the coordinates perpendicular to the defect, x and y, and since this is now a twodimensional integral, we write it as M_{2d}. Finally, the density of line defects n_{2d} is an areal density, or a number per unit area with dimensions (length)^{−2}.
It is easy to see that the same reasoning applies to planar (\(\bar n = 1\)) and point (\(\bar n = 3\)) defects. All three cases are illustrated in Fig. 2 where the scattering diagram is shown on top (analogous to an Ewald sphere) and the corresponding density of final states (Debye), \(g_{\bar n\textrm{d}}\), is given on the bottom, which for acoustic phonons obeys the following relation:
To reiterate, a phonon interacting with a point defect scatters onto a shell in k space, a phonon interacting with a line defect scatters onto a circle, and one interacting with a planar defect scatters onto two states (forward and backward scattering) on a line in k space.
Our objective in writing the rate as a product of \(n_{\bar n\textrm{d}}\), \(g_{\bar n\textrm{d}}\), and \(\overline {\left {M_{\bar n\textrm{d}}} \right^2}\), is to highlight those aspects of the answer that are most important for practical purposes. It is useful to refer to the quantities \(g_{\bar n\textrm{d}}\) and \(\overline {\left {M_{\bar n\textrm{d}}} \right^2}\) as the ‘phasespace’ and ‘matrixelement’ contributions, respectively. For scattering of acoustic phonons from dislocation strain fields (at low frequencies), the matrixelement contribution is essentially independent of frequency. Thus, its τ^{−1} ∝ ω frequency dependence^{33,34,38} comes solely from the phasespace contribution. It may also be useful to examine Eq. (1) by simple dimensional analysis. Denoting the dimensions of any quantity X by [X], we have
and Γ(k) correctly has dimensions of (time)^{−1}. It is important to note that, while the isotropic approximation is implied in Fig. 2, these dimensionality and phase space arguments hold even when anisotropy in the phonon dispersion is considered.
Dimensionality and thermal conductivity
The effects of these dimensionality arguments on the temperature dependence of the lattice thermal conductivity can be seen by applying them to standard thermal transport models, such as the Callaway model for phonon thermal conductivity (Section 4.9, Eq. (107) of ref.^{39})
in the isotropic, single mode approximation, where C_{s}(ω) is the spectral heat capacity (Supplementary Eq. (S61)) and v_{g} is the phonon group velocity. At low temperatures, when phonon scattering is dominated by microstructural defect scattering with a frequency independent matrixelement contribution, it can be found that κ_{L} varies with T as^{39}
Scattering from an infinite array of linear defects
Kinematics and diffraction conditions
Due to the wavelike nature of phonons, their interaction with periodic perturbations leads to diffraction conditions which depend on the wavelength of the phonon and the spacing of the perturbations. We now consider the case of linear defects parallel to the zaxis periodically spaced by a distance D. The x and y coordinates of the defects are
Defect arrays fitting this definition describe a variety of interfaces, such as grain boundaries and semicoherent phase boundaries which can be defined as arrays of linear dislocations^{26,27,40}.
Scattering from such an array will conserve phonon energy and momentum in the zdirection, k_{z}. In addition, diffraction conditions will be observed from the periodic structure in the y direction, such that k_{y} will change by integer multiples of 2π/D. This in turn means that for any incident phonon wavevector k, the scattered phonon wave vector k′ will take only a discrete set of values. Then, with the definition
we can solve for the final phonon states by casting the constraints on k′ as
The condition k′ = k is equivalent to k′^{2}=k^{2}, or, \({k_x^\prime}^{ 2} = k_x^2 + k_y^2  {k_y^\prime}^{2}\), which leads to
However, \(k_x^\prime\) must be real, so only a limited number of values of m are allowed for any given k, i.e. only a finite number of final phonon states (k′) exist.
Figure 3 provides a visualization of the conservation laws given in Eq. (9). Figure 3b illustrates the conservation of k_{z}, meaning the incident phonon will scatter onto a circle in k space. Figure 3c shows this scattering circle. Due to the conservation of k_{y} modulo q_{m }(as well as the conservation of energy, k′ = k), only intersections of this scattering circle with the dashed lines give valid final wavevectors. As k increases (i.e. phonon frequency increases), the size of the circle increases, while the spacing between the dashed lines is fixed. When k becomes large enough such that another term in the sum over m becomes available, a fresh diffraction event is encountered. These diffraction peaks will be observed in our calculation of GB strain field scattering.
Dimensionality crossover
When k is smaller than π/D, the only allowed solution is m = 0, for which \(k_y^\prime = k_y\), \(k_z^\prime = k_z\), and \(k_x^\prime = \pm k_x\). In other words, only forward scattering and specular reflection are allowed, and only the latter contributes to τ^{−1}. This is the solution found by Klemens when solving for phonon scattering at GBs (Eq. (73) of ref. ^{33}). In this case, the interface behaves like a structureless planar defect, and k_{y} is conserved just as k_{z}, making the final pDOS onedimensional (g_{1d}). When k is much larger than 2π/D, on the other hand, much of the scattering circle is accessible and there is effectively no constraint on \(k_y^\prime\). Now the interface behaves like a collection of independently scattering line defects, and the density of final phonon states is twodimensional (g_{2d}). The transition between these two limits gives rise to a ‘dimensionality crossover’ and has important implications for the lifetime and thermal conductivity.
We show in Supplementary Note 2 that the expression for the phonon scattering rate from an array of linear defects takes the form
where \(q_{x,m\sigma } = k_{x,m\sigma }^\prime  k_x\); \(\tilde V_1\) is the Fourier transform of the scattering potential associated with one line defect at (x, y) = (0, 0), i.e.,
and \(J({\mathbf{k}},m) = k\left( {k_x^2 + 2k_yq_m  q_m^2} \right)^{  1/2}\) is a Jacobian or volume rescaling factor associated with reexpressing the conservation laws (Eq. (9)) in terms of q_{x}, q_{y}, and q_{z}. The sum in Eq. (11) is over accessible final wavevectors as shown in Fig. 3c, and each term in the sum corresponds to a separate diffraction peak.
GB strain field scattering
In this section, we consider the specific problem of scattering from the strain field of grain boundaries, using the concepts developed in the previous two sections. An edge dislocation array (each with Burgers vector \(b\widehat {\mathbf{x}}\)) with the geometry shown in Fig. 4a is considered. This array describes a symmetric tilt grain boundary (STGB) with a misorientation angle θ_{GB} such that,
This is the same microscopic picture behind the extended Read–Shockley model which is used to describe the GB energy of many types of GBs, including GBs at high angle^{26,28}. Figure 4a schematically illustrates this interfacial defect next to its strain fields which are shown in Fig. 4b.
The displacement field u(r) and the distortion tensor ∂u_{i}/∂x_{j} are then independent of z, and the strain state can be formulated in terms of three quantities^{27},
which describe the dilation strain, shear strain, and rotation, respectively. Each type of deformation constitutes an independent scattering channel, which contributes additively to the scattering rate.
For the perturbation V due to this strain, we employ the same form as that used by Ziman (Section 6.4 of ref. ^{37}). We will take the perturbation from the array of dislocations as the sum of contributions from each individual dislocation for each deformation type. More specifically, denoting the contribution from a single dislocation along the line x = y = 0 by a subscript ‘1’ as in Eq. (11),
so that the total perturbation from each type of deformation is
Here, ω is the phonon angular frequency, and γ_{a} is a coefficient relating the type of strain or rotation a to a change in phonon energy. The change in phonon energy with strain, γ_{Δ} and γ_{S}, is defined through the generalized Grüneisen parameter (Eq. (11.75) of ref. ^{41}). The change in phonon energy with a rotation of the lattice, γ_{R}, is determined by the anisotropy of the phonon dispersion and elastic properties.
In this work, we use a single averaged Grüneisen parameter, γ = γ_{Δ} = γ_{S} = γ_{R} instead a full phononmode and deformationspecific representation, which is in line with historical treatments of Ziman^{37}, Klemens^{33}, and Carruthers^{34}, and more recent ones by Meng et al.^{42}, for example. Further discussion about the Grüneisen parameter, and extensions beyond this approximation are provided in Supplementary Note 3.
With this perturbation defined, we can now use the formalism developed in Supplementary Note 2 and Eq. (11) to calculate the phonon lifetime. It can be seen from Eq. (11) that this will require the Fourier transform of the single dislocation perturbation which can be found for each deformation type to equal
The explicit forms of these deformations are (Section 34 of ref. ^{27})
and thus their Fourier transforms are given by
where b is the Burgers vector for one dislocation, and \({\nu}\) is the Poisson ratio. Note that because all forms of \(\tilde \varepsilon _a\) scale as 1/q, and since q (the momentum transfer) scales as k = ω/v_{p}, the ω dependence cancels in \(\tilde V_{1,a}\) from Eq. (17) (at low ω). This results in a matrixelement contribution that is essentially ω independent for phononstrain field scattering, in concordance with our assertion in ‘Dimensionality and phonon scattering rate’. When the three channels are added together, we get
This expression will be averaged over incident phonon direction (Eq. (S59)) and be applied to Eq. (5) to examine its implications for κ_{L}.
Rotation and specular reflection
It leads to greater physical insight to examine the m = 0 (specular) term in the sum in Eq. (20) separately from the m ≠ 0 (nonspecular) terms. For the m = 0 term, q_{y} = 0, and we see from Eq. (19) that \(\tilde \varepsilon _{\mathrm{\Delta }} = \tilde \varepsilon _{\mathrm{S}} = 0\), so only rotation is nonzero (see the inset of Fig. 5). Thus, for k < π/D, only specular reflection survives and only rotational deformation contributes to scattering. This deformation arises because the crystals on the two sides of the GB are rotated with respect to each other, and the deformation is longranged for the same reason (see ε_{R} in Fig. 4b). The coupling coefficient for rotation is determined by the anisotropy of the crystal and is only a function of the secondorder force constants^{43}. Thus, the m = 0 term contains the same physics as the AMM, and γ_{R} can be regarded as a descriptor of anisotropy.
Phonon diffraction from GB strain fields
Scattering of wavelike phonons from the GB strain fields shown in Fig. 4 with material values for Si (given in Tables 1 and 2) is calculated using Eq. (20) and the results for phonons at normal incidence (\({\mathbf{k}}\widehat {\mathbf{x}}\)) are shown in Fig. 5.
Diffraction events for normal incidence occur when k = 2πm/D, where m is an integer, and these events appear as singularities in Γ_{gbs}. The exact position of the diffraction peaks depends on the phonon angle of incidence. This diffraction may be observable for ballistic phonons if the periodic structure of the interface is maintained for a length scale longer than the wavelengths of the phonons considered. In a real system where the GB structure is not infinitely periodic, one would expect these diffraction peaks to broaden in a manner analogous to Scherrerbroadening of Xray diffraction peaks due to particle size effects^{44}.
Dimensionality crossover in diffuse heat conduction
For diffuse (bulk) thermal conduction, a dimensionality crossover is observed as phonons transition from seeing the GB as a 2d plane, to a collection of individually scattering linear defects. In bulk thermal conduction, phonons transport diffusively, arriving at the interface in random directions rather than one specific angle of incidence. Thus, the diffraction observed for one specific k (Fig. 5) is washed out when all the possible directions of incidence are included. We define τ(ω) in Supplementary Eq. S59 as a lifetime averaged over incident direction which can be directly applied to Eq. (5). By setting Γ(k) in Eq. S59 to Γ_{gbs}(k), we obtain a directionally averaged GB strain scattering rate τ_{gbs}(ω)^{−1} which is shown in Fig. 6. This can be used to describe the ωdependence of phononGB scattering in diffuse heat conduction, and thus be used to interpret the temperature dependence of the lattice thermal conductivity of bulk polycrystalline and nanocrystalline materials.
The change in slope, or crossover in ωdependence, observed in Fig. 6 is an important result of this study. When the phonon wavelength is larger than the microscopic structure of a GB (D in this work), the phonon will see it as planar defect and the phase space contribution to the phonon lifetime will be ωindependent (g_{1d}). When the wavelength is smaller than the microscopic structure of the GB, the phonon lifetime will obtain ωdependence through the phase space contribution (g_{2d}). In the case shown above for GB strain field scattering, the matrixelement contribution is ωindependent so the ωdependence of the phonon lifetime comes exclusively from phasespace contributions. We note that, while the diffraction conditions shown in Fig. 5 require structural periodicity of the GB structure, the dimensionality crossover discussed here is purely a phasespace effect and is thus expected to be preserved even if perfect periodicity is not maintained in a real GB structure.
By recognizing the dimensionality crossover behavior, the following semiempirical expression can be inferred through careful analysis:
where
is the dimensionality crossover frequency (averaged over the incident phonon direction) and Θ(x) is the Heaviside step function. The best fit of Eq. (21) to Eq. (20) is obtained with A = 8/3 and B = 0.93 K_{ν}, where
and ν is Poisson’s ratio. Analytical justification of the dependencies, functional form, and magnitudes of coefficients A and B in Eq. (21) is given in Supplementary Note 2. Eq. (21) provides an excellent approximation (dashed lines in Figs. 6 and 7) for the numerical solution of the full analytical expression in Eq. (20) (solid lines). We note that the first term in Eq. (21) is the m = 0 (specular) term in the sum in Eq. (20). It is ωindependent and proportional to the linear density of interfaces n_{1d}, a misorientation factor b/D (Eq. (13)), and a coefficient characterizing the crystal anisotropy γ_{R}. The second term in Eq. (21) contains m≠0 (nonspecular) terms and is proportional to the areal density of GB dislocations n_{1d}/D and the Burgers vector squared b^{2}, and a coefficient characterizing the anharmonicity of the crystal γ. These dependencies stem directly from the dimensionality arguments presented while discussing Figs. 2 and 3. As discussed in ‘Rotation and specular reflection’, the first term in Eq. (21) depends only on rotation, while the second term depends on rotation, hydrostatic, and shear strain. Thus, if the scattering coefficients of each deformation type (a = Δ, S, R) are treated separately the relative magnitudes of the first and second term will change and the dependence of \(\tau _{{\mathrm{gbs}}}^{  1}\) with GB angle will also change.
The scattering theory presented here characterizes the phonon GB interaction as a phonon lifetime τ(ω), which is a convenient way to understand dimensionality and phase space effects. In Fig. 6c we cast our results in the form of a spectral phonon transmissivity using the expression provided by Dames and Chen^{45}
This demonstrates how the dimensionality crossover of the phononinterface interaction results in a transmissivity that is ωindependent at low ω, and decreases above the critical frequency ω^{*}, which is a function of the linear defect spacing.
LowT thermal conductivity of polycrystals
Now, we discuss how GB strain scattering influences thermal transport in polycrystalline materials. Specific analysis is given for polycrystalline Si, AlN, and Al_{2}O_{3}. We use the Callaway model for phonon thermal conductivity (Eq. (5)) and modeling procedure given by Wang et al.^{12,46} wherein the net relaxation rate is given by
The three contributions are due to phonon–phonon (τ_{pp}), intrinsic point defect (τ_{pd}) and GB strain (τ_{gbs}) scattering. We take \(\tau _{{\mathrm{pp}}}^{  1} = C_1\omega ^2Te^{  C_2/T}\) (same form as that given by Slack^{47}), \(\tau _{{\mathrm{pd}}}^{  1} = C_3\omega ^4\), but account for GB scattering in polycrystalline materials using Eq. (21). Since \(\tau _{{\mathrm{pp}}}^{  1}\) and \(\tau _{{\mathrm{pd}}}^{  1}\) are considered intrinsic to a given crystal system, the coefficients C_{1}, C_{2}, and C_{3} are fit to single crystal data (Table 1) and fixed for subsequent modeling. The parameters for Si are the same as those of Wang et al.^{12}.
In Fig. 7, we show the temperature dependence of κ_{L} that results from the modeling procedure described above for the specific case of Si. This dependence is shown for various values of D, the GB dislocation spacing (Fig. 4a), with the remaining material parameters for Si given in Table 2. The central point of the figure is that depending on D, the T dependence of κ_{L} at low temperature (below the temperature of maximum κ_{L}) can vary from T^{2} to T^{3}. At such temperatures the dominant scattering in this model is from GB strain and therefore, the variation from T^{2} to T^{3} stems directly from the dimensionality crossover argument embedded in our semiempirical formula for τ_{gbs} (Eq.(21), Fig. 6). As GB dislocation spacing decreases, the crossover frequency ω^{*} (Eq. 22) increases. For reference, the peak in the phonon occupation number at ~50 K occurs at \(\omega /\omega _{\mathrm{D}} \simeq 0.2\). For the case of D = 1 nm, ω^{*}/ω_{D} = 0.37, so below 50 K most phonons see the GB as a planar defect with \(\bar n = 1\) (τ independent of ω) resulting in κ_{L} ∝ T^{3} (see lower most curve in Fig. 7). For larger dislocation spacings the crossover shifts downward in frequency and a significant number of phonons see the GB as a collection of linear defects with \(\bar n = 2\) and τ^{−1} ∝ ω, leading to κ_{L} ∝ T^{2}. This crossover in τ^{−1} also means that for any fixed D there is a transition from κ_{L} ∝ T^{2} to κ_{L} ∝ T^{3} at a crossover temperature which is related to ω^{*}.
We now wish to compare our model for GB strain scattering with experimental thermal conductivity data of real materials. We choose polycrystalline Si^{12}, AlN^{13}, and Al_{2}O_{3}^{14} as model systems. The data for AlN given by Watari et al. is specifically included because the sample was synthesized with clean GBs with almost no GB oxide phase. The intrinsic phonon scattering parameters are given in Table 1 as before. In addition, material parameters related to GB strain scattering are required to calculate τ_{gbs}. These parameters are given in Table 2 and are obtained as follows. Literature values are used for the average speed of sound, Grüneisen parameter, and Poisson’s ratio. When applied to a bulk polycrystal, τ_{gbs} in Eq. (21) is meant to embody phonon scattering off an ensemble of GB structures within the polycrystal. Thus, one may interpret D as the characteristic length scale of GB structure in the polycrystal and b as an average GB dislocation Burgers vector. Recognizing the energetic considerations which require dislocations to have Burgers vectors which are integer multiples of a primitive unit cell vector (see Figure 9–2 in ref. ^{27}), a good approximation (and lower bound) for the average GB Burgers vector is b_{GB} = (VN)^{1/3}, where V is the volume per atom and N is the number of atoms in the primitive unit cell. When chosen in this way, b_{GB} is fixed and the only adjustable parameters are D, and the average grain size \(\bar d\). The latter is related to the linear density of interfaces by calculating the GB area over volume assuming cubic grains, i.e., \(n_{1{\mathrm {d}}} = 3/\bar d\). The agreement between the experimental grain sizes and the values used in this modeling study is reasonable, as can be seen in Table 2.
The results of this comparison are shown in Fig. 8. The figure includes data for both single and polycrystalline materials. The single crystal data of AlN and Al_{2}O_{3} show classic T^{3} power laws at lowT, indicative of Casimir scattering from crystal surfaces. Thus, in the theoretical modeling, ωindependent Casimir scattering is incorporated by adding a term \(\tau _{{\mathrm{Casimir}}}^{  1} = v_{\mathrm{g}}/L_{{\mathrm{sc}}}\) in the total scattering rate. Here, L_{sc} is the size of the single crystal (Table 1). By contrast, all polycrystalline data show T^{2} dependence at lowT. This dependence is captured by our GB strain scattering model and demonstrates the importance of defect dimensionality considerations. The figures also show a comparison of the data with the commonly used gray model, where instead of using \(\tau _{{\mathrm{gbs}}}^{  1}\) in Eq. (25) we use \(\tau _{{\mathrm{gray}}}^{  1} = v_{\mathrm{g}}/\bar d\). As discussed in the Introduction τ_{gray} is ωindependent (like the AMM and DMM at low temperatures) since it is a direct extension of Casmir scattering to polycrystals and thus predicts a T^{3} power law which is not seen. In addition, the lowT magnitude of κ_{L} given by the gray model is too low by several orders of magnitude. We note that the value of \(\bar d\) used to produce the dashed lines in Fig. 8 is adjusted to match the magnitude of the rollover κ_{L}. This value differs from that shown in Table 2 by at most a factor of two. Were this adjustment not made the comparison with experimental data would be worse. We note here that for the theoretical modeling we have used both Debye and Bornvon Karman (BvK) dispersions (Supplementary Note 4) and as can be seen the differences are not significant except for the softest material considered here, Si. In particular the lowT power law behavior is not affected when dispersive phonons are considered.
The characteristic length scale parameter D deserves further discussion. We can understand the values used in our theoretical model by considering the case of Si. The modeling results show that GBs with characteristic lengths of \(D \gtrsim 3\,{\kern 1pt} \,{\mathrm{nm}}\) will display κ_{L} ∝ T^{2} like behavior above ~15 K, as is observed experimentally. By relating D to a GB angle using Eq. (13), we can estimate that GBs within 5 to 10° of a special boundary should have spacings larger than ~3 nm. This includes lowangle GBs, as well as GBs in the vicinity of special GBs at higher angle (e.g. Σ5 at 36.9° for symmetric tilt and twist boundaries in cubic materials)^{19,20,21}. Given that this window spans a significant range of possible GB angles, and that such GBs are low in energy^{26}, we argue that a sufficient proportion of GBs that occur naturally in a polycrystalline material would scatter with τ^{−1} ∝ ω, and result in κ_{L} ∝ T^{2}. While the results of this modeling study agree with the experimental data available, controlled computation and experimental studies containing spectral information of the phonon–GB interaction would help further validate the effects discussed here.
Structural information of interfaces can indeed be included when calculating the thermal boundary resistance by computational methods, such as molecular dynamics^{48} or Green’s function methods^{49,50}, and much progress has been made regarding these approaches in recent years^{3}. These detailed methods are invaluable for progress in the field of heat transfer as the interfacial structure can be defined and systemically controlled, and spectral information can be obtained which is difficult to obtain experimentally^{51}. Due to the inevitable complexity of interfaces in real materials (e.g. the GB character distribution in a bulk polycrystal), detailed theoretical and computational treatments should be used to establish engineering design principles which are generalizable and can thus be applied to real systems. This work shows, through standard scattering theory, that general kinematic arguments can explain measurable phenomena which emerge from this complexity. We hope this work can help guide more detailed computational simulations and experiments.
Phonondislocation interactions have also been studied using molecular dynamics^{52}, and even ab initio methods^{53}. The ab initio technique of Wang et al.^{53} extends the Tmatrix formalism to phonon scattering on an array of dislocation quadrupoles, with the periodicity imposed by periodic boundary conditions^{53}. The structure calculated in ref. ^{53} however eliminates the long range (1/r) strain field^{54} which is characteristic of dislocations and is known to be the dominant phonondislocation interaction^{37,38,43,55,56,57}. This long range strain field is required to give the τ^{−1} ∝ ω and thus κ_{L} ∝ T^{2}, so it is not surprising that this study does not find κ_{L} ∝ T^{2}. We emphasize that the dislocation configuration considered in ref. ^{53} does not describe a GB, and since it does not contain the 1/r strain field it does not describe isolated lattice dislocations.
Discussion
Phonon scattering at interfaces is an inherently complex phenomenon where many physical processes are at play simultaneously. This work focuses specifically on effects that arise when considering interfacial structure at the nanoscale by defining the interface as an array of linear defects, rather than treating the interface as a structureless planar defect. This definition is sufficiently general such that it includes many types of grain boundaries (particularly those of low energy) and semicoherent phase boundaries. Indeed the interface between two materials with structural periodicity will tend to have structural periodicity itself, and we suggest that the standard model for phononinterface scattering in crystalline materials should not assume perfect disorder at the interface. Several emergent phenomena arise from this analysis stemming directly from this structural definition. These include phonon diffraction conditions arising from the periodic structure of the interface and the wavelike nature of phonons, as well as a crossover in the ω dependence of the phonon lifetime stemming from dimensionality and phase space considerations. The general analytical expression derived was applied to the specific case of a symmetric tilt GB where the linear defects were defined as the strain field from edge dislocations. The result is a phononGB strain lifetime (τ_{gbs}) that is independent of ω below a critical frequency \(\omega ^ \ast \simeq 4\pi v_{\mathrm{s}}/3D\) which depends on the GB dislocation spacing D, and \(\tau _{{\mathrm{gbs}}}^{  1} \propto \omega\) above ω^{*}. A simple semiempircal expression is provided as an excellent approximation of the full analytical expression, which embodies this dimensionality crossover effect. This scattering theory is applied to standard phonon transport models and is shown to explain the κ_{L} ∝ T^{2} temperature dependence of polycrystalline materials at low temperatures. This power law analysis provides evidence that the dominant phonon GB scattering mechanism is through GB strain fields and that interfacial structure and strain energy are important.
Code availability
The Mathematica scripts used for numerical computation in this study are provided at https://github.com/rileyhanus/Phononscatteringandtransportinpolycyrstals.
Data availability
The literature data used in this study are compiled at https://github.com/rileyhanus/Phononscatteringandtransportinpolycyrstals.
References
 1.
Mei, S. et al. Boundaries, interfaces, point defects, and strain as impediments to thermal transport in nanostructures. IEEE 1–10 (2017).
 2.
Pop, E. Energy dissipation and transport in nanoscale devices. Nano Res. 3, 147–169 (2010).
 3.
Monachon, C., Weber, L. & Dames, C. Thermal boundary conductance: a materials science perspective. Annu. Rev. Mater. Res. 46, 433–463 (2016).
 4.
Soyez, G. et al. Grainsizedependent thermal conductivity of nanocrystalline yttriastabilized zirconia films grown by metalorganic chemical vapor deposition. Appl. Phys. Lett. 77, 1155–1157 (2000).
 5.
Rauf, A., Yu, Q., Jin, L. & Zhou, C. Microstructure and thermal properties of nanostructured lanthanadoped yttriastabilized zirconia thermal barrier coatings by air plasma spraying. Scr. Mater. 66, 109–112 (2012).
 6.
Kim, S. I. et al. Dense dislocation arrays embedded in grain boundaries for highperformance bulk thermoelectrics. Science 348, 109–115 (2015).
 7.
Zong, P.a et al. Skutterudite with graphenemodified grainboundary complexion enhances zT enabling highefficiency thermoelectric device. Energy Environ. Sci. 10, 183–191 (2017).
 8.
Cahill, D. G. et al. Nanoscale thermal transport. II. 2003–2012. Appl. Phys. Rev. 1, 1–45 (2014).
 9.
Little, W. A. Transport of heat between dissimilar solids at low temperatures. Candian J. Phys. 37, 334–349 (1959).
 10.
Swartz, E. T. & Pohl, R. O. Thermal boundary resistance. Rev. Mod. Phys. 61, 605–668 (1989).
 11.
Casimir, H. B. G. Note on the conduction of heat in crystals. Physica 5, 495–500 (1938).
 12.
Wang, Z., Alaniz, J. E., Jang, W., Garay, J. E. & Dames, C. Thermal conductivity of nanocrystalline silicon: importance of grain size and frequencydependent mean free paths. Nano Lett. 11, 2206–2213 (2011).
 13.
Watari, K. et al. Thermal conductivity of AlN ceramic with a very low amount of grain boundary phase at 4 to 1000 K. J. Mater. Res. 17, 2940–2944 (2002).
 14.
Berman, R. The thermal conductivity of some polycrystalline solids at low temperatures. Proc. Phys. Soc. Sect. A 65, 1029–1040 (1952).
 15.
Hori, T., Shiomi, J. & Dames, C. Effective phonon mean free path in polycrystalline nanostructures. Appl. Phys. Lett. 106, 1–6 (2015).
 16.
Hua, C. & Minnich, A. J. Importance of frequencydependent grain boundary scattering in nanocrystalline silicon and silicongermanium thermoelectrics. Semicond. Sci. Technol. 29, 1–17 (2014).
 17.
Oyake, T. et al. Ultimate confinement of phonon propagation in silicon nanocrystalline structure. Phys. Rev. Lett. 120, 45901 (2018).
 18.
Hua, C., Chen, X., Ravichandran, N. K. & Minnich, A. J. Experimental metrology to obtain thermal phonon transmission coefficients at solid interfaces. Phys. Rev. B 95, 205423 (2017).
 19.
Balluffi, R. W., Komem, Y. & Schober, T. Electron microscope studies of grain boundary dislocation behavior. Surf. Sci. 31, 68–103 (1971).
 20.
Schober, T. Observation of misfit dislocation arrays in high angle (110) twist grain boundaries in gold. Philos. Mag. 22, 1063–1068 (1970).
 21.
Schober, T. & Balluffi, R. W. Quantitative observation of misfit dislocation arrays in low and high angle twist grain boundaries. Philos. Mag. 21, 109–123 (1970).
 22.
von Alfthan, S., Haynes, P. D., Kaski, K. & Sutton, A. P. Are the structures of twist grain boundaries in silicon ordered at 0 K? Phys. Rev. Lett. 96, 1–4 (2006).
 23.
von Alfthan, S. et al. The structure of grain boundaries in strontium titanate: theory, simulation, and electron microscopy. Annu. Rev. Mater. Res. 40, 557–599 (2010).
 24.
Read, W. T. & Shockley, W. Dislocation models of crystal grain boundaries. Phys. Rev. 78, 275–289 (1950).
 25.
Priester, L. Grain Boundaries From Theory to Engineering (Springer, Dordrecht 2006).
 26.
Wolf, D. Structure and energy of grain boundaries. In Handbook of Materials Modelling, ed.: Yip, Sidney. Springer Netherlands: Dordrecht, chap. 6.9, 1953–1983 (2005).
 27.
Hirth, J. & Lothe, J. Theory of Dislocations, 2nd edn (Malabar, FL, Krieger Publishing Company 1982).
 28.
Watanabe, T., Ni, B., Phillpot, S. R., Schelling, P. K. & Keblinski, P. Thermal conductance across grain boundaries in diamond from molecular dynamics simulation. J. Appl. Phys. 102, 063503 (2007).
 29.
Huang, S. H. et al. Strain relief by periodic misfit arrays for low defect density GaSb on GaAs. Appl. Phys. Lett. 88, 131911 (2006).
 30.
Yastrubchak, O. et al. Misfit dislocations and surface morphology of latticemismatched GaAs/InGaAs heterostructures. Phys. E: Low.Dimens. Syst. Nanostruct. 17, 561–563 (2003).
 31.
Balluffi, R. W., Sass, S. L. & Schober, T. Grain boundary dislocation networks as electron diffraction gratings. Philos. Mag. 26, 585–592 (1972).
 32.
Kaganer, V. M., Köhler, R., Schmidbauer, M., Opitz, R. & Jenichen, B. Xray diffraction peaks due to misfit dislocations in heteroepitaxial structures. Phys. Rev. B 55, 1793–1810 (1997).
 33.
Klemens, P. G. The scattering of lowfrequency lattice waves by static imperfections. Proc. Phys. Soc. Sect. A 68, 1113–1128 (1955).
 34.
Carruthers, P. Scattering of phonons by elastic strain fields and the thermal resistance of dislocations. Phys. Rev. 114, 995–1001 (1959).
 35.
Omini, M. & Sparavigna, A. Role of grain boundaries as phonon diffraction gratings in the theory of thermal conductivity. Phys. Rev. B 61, 6677–6688 (2000).
 36.
Kim, H.S., Kang, S. D., Tang, Y., Hanus, R. & Jeffrey Snyder, G. Dislocation strain as the mechanism of phonon scattering at grain boundaries. Mater. Horiz. 3, 234–240 (2016).
 37.
Ziman, J. M. Electrons and Phonons: The Theory of Transport Phenomena in Solids (Oxford University Press, New York 1960).
 38.
Brown, R. The effect of dislocations on thermal conductivity. J. Phys. Colloq. 42, C6–271–C6–273 (1981).
 39.
Kaviany, M. Heat Transfer Physics. 1st edn, (Cambridge Universtiy Press, New York, 2008).
 40.
Merwe, J. H. V. D. On the stresses and energies associated with intercrystalline boundaries. Proc. Phys. Soc. Sect. A 63, 616–637 (2002).
 41.
Wallace, D. C. Thermodynamics of Crystals. (John Wiley and Sons, Inc., New York, 1972).
 42.
Meng, Q., Wu, L. & Zhu, Y. Phonon scattering of interfacial strain field between dissimilar lattices. Phys. Rev. B  Condens. Matter Mater. Phys. 87, 1–9 (2013).
 43.
Brown, R. A. The scattering of phonons by the strain and rotation fields of crystal defects. J. Phys. C: Solid State Phys. 16, 1009–1029 (1983).
 44.
Cullity, B. & Stock, S. Elements of XRay Diffraction. 3rd edn (Pearson Education, Cambridge, 2014).
 45.
Dames, C. & Chen, G. Theoretical phonon thermal conductivity of Si/Ge superlattice nanowires. J. Appl. Phys. 95, 682–693 (2004).
 46.
Hanus, R. GitHub Repository https://github.com/rileyhanus/Phononscatteringandtransportinpolycyrstals (2018).
 47.
Slack, G. A. & Galginaitis, S. Thermal conductivity and phonon scattering by magnetic impurities in CdTe. Phys. Rev. 133, A253–A268 (1964).
 48.
Schelling, P. K., Phillpot, S. R. & Keblinski, P. Kapitza conductance and phonon scattering at grain boundaries by simulation. J. Appl. Phys. 95, 6082–6091 (2004).
 49.
Polanco, C. A. et al. Role of crystal structure and junction morphology on interface thermal conductance. Phys. Rev. B—Condens. Matter Mater. Phys. 92, 1–10 (2015).
 50.
Sadasivam, S. et al. The atomistic Green’s funciton method for interfacial phonon transport. Annu. Rev.Heat Transf. 17, 89–145 (2014).
 51.
Sääskilahti, K., Oksanen, J., Tulkki, J. & Volz, S. Role of anharmonic phonon scattering in the spectrally decomposed thermal conductance at planar interfaces. Phys. Rev. B—Condens. Matter Mater. Phys. 90, 1–8 (2014).
 52.
Deng, B., Chernatynskiy, A., Shukla, P., Sinnott, S. & Phillpot, S. Effects of edge dislocations on thermal transport in UO_{2}. J. Nucl. Mater. 434, 203–209 (2013).
 53.
Wang, T., Carrete, J., Van Roekeghem, A., Mingo, N. & Madsen, G. K. H. Ab initio phonon scattering by dislocations. Phys. Rev. B 95, 1–7 (2017).
 54.
Moore, J. & KuhlmannWilsdorf, D. Theory of dislocation cells. II. Dislocation multipoles. J. Appl. Phys. 42, 953–961 (1971).
 55.
Friedel, J. Dislocations (New York, Pergamon Press 1964).
 56.
Sato, M. & Sumino, K. Effect of dislocations on the low temperature thermal conductivity in germanium. J. Phys. Soc. Jpn. 36, 1075–1083 (1974).
 57.
Zhu, D.m & Anderson, A. C. Scattering of phonons by sessile dislocations in deformed germanium. J. Low. Temp. Phys. 82, 37–47 (1991).
 58.
Glassbrenner, C. J. & Slack, G. A. Thermal conductivity of silicon and germanium from 3 K to the melting point. Phys. Rev. 134, A1058–A1069 (1964).
 59.
Morkoç H. General properties of nitrides. In Nitride Semiconductor Devices, Vol. 1 1–61 (WileyVCH, Weinheim, Germany, 2013).
 60.
Rossi, LouisR. & Lawrence, WillisG. Elastic properties of oxide solid solutions: the system Al_{2}O_{3}–Cr_{2}O_{3}. J. Am. Ceram. Soc. 53, 604–608 (1970).
 61.
Rücker, H. & Methfessel, M. Anharmonic keating model for groupIV semiconductors with application to the lattice dynamics in alloys of Si, Ge, and C. Phys. Rev. B 52, 11059–11072 (1995).
 62.
Iwanaga, H., Kunishige, a & Takeuchi, S. Anisotropic thermal expansion in wurtzitetype crystals. J. Mater. Sci. 35, 2451–2454 (2000).
 63.
GarcíaRevilla, S., Rodríguez, F., Valiente, R. & Pollnau, M. Optical spectroscopy of Al_{2}O_{3}:Ti^{3+} single crystal under hydrostatic pressure. The influence on the Jahn–Teller coupling. J. Phys.: Condens. Matter 14, 447–459 (2002).
 64.
Wortman, J. J. & Evans, R. A. Young’s modulus, shear modulus, and poisson’s ratio in silicon and germanium. J. Appl. Phys. 36, 153–156 (1965).
Acknowledgements
G.J.S. and R.H. acknowledge EFRC SolidState SolarThermal Energy Conversion Center (S3TEC) Grant DESC0001299. R.H. acknowledges support from the Johannes and Julia Randall Weertman Graduate Fellowship.
Author information
Affiliations
Contributions
R.H. and G.J.S. initiated the study. R.H. and A.G. developed the mathematical theory and modeling. R.H. drafted the manuscript. R.H., G.J.S., and A.G. revised the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Hanus, R., Garg, A. & Snyder, G.J. Phonon diffraction and dimensionality crossover in phononinterface scattering. Commun Phys 1, 78 (2018). https://doi.org/10.1038/s420050180070z
Received:
Accepted:
Published:
Further reading

Probing the phonon mean free paths in dislocation core by molecular dynamics simulation
Journal of Applied Physics (2021)

Enhanced thermoelectric performance of chalcopyrite nanocomposite via comilling of synthetic and natural minerals
Materials Letters (2020)

GaN thermal transport limited by the interplay of dislocations and size effects
Physical Review B (2020)

Revealing nanochemistry at lattice defects in thermoelectric materials using atom probe tomography
Materials Today (2020)

Transition across a sharp interface: Data from Raman and Brillouin imaging spectroscopy
Data in Brief (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.